Pré-visualização3 páginas

NumerIcAl SImulAtIoN ANd INduStrIAl PrActIce of INcluSIoN removAl from molteN Steel by GAS bottom- blowING IN coNtINuouS cAStING tuNdISh Z. meijie, G. huazhi, h. Ao, Z. hongxi and d. chengji Wuhan University of Science and Technology, the Hubei Province Key Laboratory of Refractories and Ceramics, Wuhan 430081, China (Received 20 January 2011; accepted 20 April 2011) Abstract Gas blowing at the bottom of tundish is an efficient metallurgy technique in clean steelmaking. In this paper, the removal of small size inclusions in the gas bottom-blowing tundish was studied by numerical simulation and industrial practice. The residence time distribution (RTD) of molten steel in the tundish was calculated by mathematical modeling. The content of small size inclusions in the slab was analyzed using a oxygen probing and metallographic images. The results show that the molten steel characteristics obviously change when applied gas bottom-blowing, the average residence time of molten steel in the tundish prolongs more than 100s and the dead volume fraction decreases about 5%. Therefore, the removal efficiency of small size inclusions greatly increases because of bubbles attachment and long moving path. Industrial experiment results show that the average inclusions content of less than 20\u3bcm decreases more than 24%, the average overall oxygen content decreases about 15% when controlling the reasonable blowing parameters. Keywords: Tundish; Inclusion removal; Gas blowing; Modeling; Industrial practice. # Corresponding author: major6886@gmail.com J o u r n a l o f M i n i n g a n d M e t a l l u r g y J. Min. Metall. Sect. B-Metall. 47 (2) B (2011) 137 - 147 1. Introduction The tundish plays an important role in clean steel making by removing some unwanted inclusions from molten steel. So, various kinds of flow control devices (FCD), such as dam, weir, baffles and turbulence inhibitor (TI) have been developed in recent decades [1-3]. In addition, some new methods have also been proposed in continuous casting process including plasma heating for maintaining appropriate casting DOI:10.2298/JMMB11012006M steel temperature [4,5], centrifugal flow tundish [6], swirling flow tundish [7] and gas bottom-blowing [8-10]. In these renovations, gas bottom-blowing has attracted more attentions because of higher removal efficiency for small size particle inclusions and low investment. The inert gas was injected through porous brick at the bottom of tundish. Gas bubble curtains are formed. Wei et al [11] have demonstrated through the cold model study that when the particles are not wetted by the liquid, they can be captured by gas bubbles and floated up to the free surface. Solid inclusions such as alumina and silica are not wetted by the liquid steel and therefore can be removed by attachment to gas bubbles. Wang et al [12] have developed a mathematical model to determine the optimum bubble size for the removal of inclusions from molten steel by floation. The model suggests that the optimum bubbles sizes for the removal from steel of alumina inclusions smaller than 50×10-6 m in size are in the range of 0.5 to 2×10-3 m in diameter. On the basis of studies of particle-gas intercation in water based mineral processing systems, Lifeng Zhang and S. Taniguchi [13] discussed the mechanism of inclusion removal by bubbles. The overall process of inclusion floation in steel by a gas bubble can be divided into subprocessed: (1) approach of a bubble to an inclusion; (2) formation of a thin liquid film between inclusion and bubble; (3) oscillation and / or sliding of the inclusion on the bubble surface; (4) drainage and rupture of the film with the formation of a dynamic three-phase contact; (5) stabilisation of the bubble- inclusion aggregate with respect to external stresses; (6) flotation of the bubble-inclusion aggregate. Then a simple mathematical model of inclusion removal by bubble flotation was described. The contribution of gas bubbling curtains in the tundish to the removal of small size particles has been verified by physical and mathematical modeling [14-16]. In this subject, the flow field, RTD curves and inclusion removal efficiency were analyzed by mathematical modeling at first, then the industrial experience was experimented in Laiwu IRON and Steel Lmtd. The average Z. Meijie / JMM 47 (2) B (2011) 137 - 147138 Fig. 1. Geometric dimensions of the industrial tundish contents of overall oxygen and small size (<20\u3bcm) inclusions were detected. 2. description of the industrial tundish The selected tundish for the present analysis is a 30t tundish of Lai Wu Iron & Steel Ltd., China. The dimensions of this tundish is shown in Figure 1. This two-strand tundish was equipped with a turbulence inhibitor (TI) and a pair of baffles whose dimensions were shown in Figure 2 and Figure 3 respectively. Under steady state conditions, the liquid steel depth in the tundish is 0.96m. The inner diameters of ladle shroud and submerged nozzle are 70mm and 50mm respectively. The numerical simulation was performed for casting slabs (175×1260mm) with casting speed 1.4m·min-1. In order to study the effect of gas bottom- blowing on removal of inclusions, a pair of porous plugs were established on the bottom of the tundish. Dimensions of the plug were shown in Figure 4. 2.1. mathematical model control equations. A three-dimensional, steady, turbulent bubbly flow in the tundish Z. Meijie / JMM 47 (2) B (2011) 137 - 147 139 Fig. 2. Geometric dimensions of the TI Fig. 4. Schematic of gas curtain bricks for industrial tundish Fig. 3. Geometric dimensions of the baffle was simulated using the Eulerian-Eulerian two-phase flow model[10], which molten steel was considered as the primary phase and gas as the secondary phase. The continuity and momentum equations for each phase were solved together with the standard k-\u3b5turbulent model for liquid steel. The Porous media model was used for gas flow through the porous brick [17]. The viscous resistance factor and inertial resistance factor of gas flow through the brick were acquired by the method for measuring permeability of refractory products [18, 19]. The equation for residence time distribution (RTD) is a normal species transportation equation. Inclusion trajectories were calculated using the discrete phase model (DPM) which solves a transport equation for each inclusion particle as it travels through the previously calculated, steady-state, flow field of molten steel and argon gas. 2.2. boundary conditions The boundary conditions for momentum transfer to all solid surfaces, including walls and bottom of tundish, surfaces of baffles and TI were those of non-slipping. Wall functions described by Anderson [20] are used at nodes close to all solid walls. The interface of slag and molten steel is considered as free surface. Velocity gradients, turbulent kinetic energy and its dissipation rate were assumed zero on the free surface and at all solid surfaces. At the liquid inlet, a uniform normal velocity profile was assumed and the average velocity was fixed according to the flow rate. k and \u3b5 were specified using the semi-empirical equations [21]. Outflow was set at the liquid outlet. The density and viscosity of molten steel were assumed constants: 6940kg/m3 and 0.06239Pa·s. At the gas inlet, the gas injection superficial velocity was specified from the gas flow rate and the region area of porous refractory, the liquid volume fraction was set as zero. According to the water modeling and past research works [14, 22], the bubbles were assumed as spherical shape and their diameters were assumed as 2mm. The density and viscosity of hot argon gas were assumed constants: 0.342kg/m3 and 5.741e- 05 Pa·s. Ideal absorption was assumed at the top surface. At the tundish wall, only a part of inclusions were adopted. Inclusions were assumed